Salt-stone Oxidation Study: Leaching Method - 13092

Cementitious waste forms can be designed to chemically stabilize selected contaminants, such as Tc{sup +7} and Cr{sup +6}, by chemically reduction to lower valance states, Tc{sup +4} and Cr{sup +3}, respectively, and precipitation of these species in alkaline media as low solubility solid phases. Data for oxidation of this type of cementitious waste form cured under field conditions as a function of time is required for predicting the performance of the waste form and disposal facility. The rate of oxidation (oxidation front advancement) is an important parameter for predicting performance because the solubilities of some radionuclide contaminants, e.g., technetium, are a function of the oxidation state. A non-radioactive experiment was designed for quantifying the oxidation front advancement using chromium, as an approximate redox-sensitive surrogate (Cr{sup +6} / Cr{sup +3}) for technetium (Tc{sup +7} / Tc{sup +4}). Nonradioactive cementitious waste forms were prepared in the laboratory and cured under both laboratory and 'field conditions'. Laboratory conditions were ambient temperature and sealed sample containers. Field conditions were approximated by curing samples in open containers which were placed inside a plastic container stored outdoors at SRS. The container had a lid and was instrumented with temperature and humidity probes. Sub-samples as thin asmore » 0.2 mm were taken as a function of distance from the exposed surface of the as-cast sample. The sub-samples were leached and the leachates were analyzed for chromium, nitrate, nitrite and sodium. Nitrate, nitrite, and sodium concentrations were used to provide baseline data because these species are not chemically retained in the waste form matrix to any significant extent and are not redox sensitive. 'Effective' oxidation fronts for Cr were measured for samples containing 1000, 500 and 20 mg/kg Cr added as soluble sodium chromate, Na{sub 2}CrO{sub 4}. For a sample cured for 129 days under field conditions, leachable Cr (assumed to be the oxidized form, i.e., Cr{sup +6} was detected in the top 15 to 20 mm of the sample spiked with 1000 mg/kg Cr. Below about 20 mm, the Cr concentrations in leachates were below the detection limit (< 0.010 mg/L) which indicates that the oxidation as the result of exposure to air was limited to the top 20 mm of the sample after exposure for 129 days and that the bulk of the waste form was not affected, i.e., the Cr was stabilized and insoluble. For samples cured in the laboratory, leachable Cr was detected in the top 8 mm of the Cr 1000 sample cured in the laboratory for 37 days. Between 8 and 14 mm, the concentration Cr in the leachate dropped by a factor of about 20 to just above the detection limit. These depth of penetration results indicate that the rate of advancement of the oxidation front for samples spiked with 1000 mg/kg Cr cured under 'field conditions' for 129 days is less than that for the sample cured in the laboratory for 37 days, i.e., 0.156 and 0.216 mm/day, respectively. Additional data are presented for samples spiked with 500 and 20 mg/kg Cr. In summary, cementitious waste forms are porous solids with a network of interconnected pores ranging in diameter from 10 E-10 m to greater than a few mm. The oxidation process is assumed to occur as the result of oxygen transport through the interconnected porosity which may be filled with air, aqueous salt solution, or both. Upon oxidation, the Cr becomes soluble and can be transported in solution through aqueous pore fluid or leachate. (authors)« less